# Contact-free measurement and numerical and analytical evaluation of the strain distribution in a wood-FRP lap-joint

←

**Page content transcription**

If your browser does not render page correctly, please read the page content below

Materials and Structures DOI 10.1617/s11527-009-9568-x ORIGINAL ARTICLE Contact-free measurement and numerical and analytical evaluation of the strain distribution in a wood-FRP lap-joint Johan Vessby • Erik Serrano • Bertil Enquist Received: 8 May 2009 / Accepted: 26 November 2009 Ó RILEM 2009 Abstract Wood specimens to each of which a anchorage length in a non-linear fashion. The exper- laminate of carbon fibre reinforcement polymers imental, analytical and numerical results were shown (FRP) was glued (creating a lap joint in each case) to be in close agreement with respect to the strength were loaded to failure. A total of 15 specimens of and the strain distribution obtained. three types differing in the glued length (anchorage length) of the FRP laminate (50, 150 and 250 mm Keywords FRP Lap-joint Volkersen Wood respectively) were tested, their strength, stiffness and strain distribution being evaluated. Synchronized digital cameras (charge-coupled devices) used in 1 Background testing enabled strain fields on surfaces they were directed at during the loading procedure to be In the building sector, enhancement of the load- measured. These results were also evaluated both carrying capacity of new or already existing structures analytically on the basis of generalized Volkersen without any change in their geometry needing to be theory and numerically by use of the finite element made may be sought. This may be based on changed method. The lap joints showed a high level of conditions, such as an increase in loading due to stiffness as compared with mechanical joints. A high rebuilding or redesigning of the overall structure. degree of accuracy in the evaluation of stiffness was Points in close proximity to connections between achieved through the use of the contact-free evalu- different building elements or around holes or notches ation system. The load-bearing capacity of joints of in beams, for example, can be in particular need this type was found to be dependent upon the of reinforcement. What is aimed at may be greater stiffness, enhanced load-bearing capacity, or both. One method of increasing the stiffness and strength of J. Vessby a structure is by use of Fibre Reinforced Polymers Tyréns, Storgatan 40, 352 31 Växjö, Sweden (FRP). These show a very high level of strength and stiffness as compared with many other materials. J. Vessby (&) E. Serrano B. Enquist Växjö University, Lückligs Plats 1, 351 95 Växjö, Sweden The aim of the present study was to investigate e-mail: johan.vessby@vxu.se experimentally under well-defined conditions and E. Serrano evaluate analytically and numerically the properties e-mail: erik.serrano@vxu.se of the interaction between FRP-laminates (referred to B. Enquist hereafter as FRPs) and timber to which they are glued e-mail: bertil.enquist@vxu.se to form single-overlap joints (these are also termed

Materials and Structures lap-joints). Other researchers, such as Gustafsson and [mm] Enquist [1], Johansson et al. [2] and Kliger et al. [3] have reported both experimentally and numerically Indicates the fibre based findings concerning properties of the FRP- 145 orientation of the wood timber interaction. In these studies no use was made of 70 and FRP respectively. a contact-free evaluation system to examine in detail Wood 350 the behaviour of the joint, a matter the very large amount of data obtained by use of such a system makes FRP possible. Guan et al. [4] studied a timber beam Part of the timber where reinforced with glass fibre pretensioned to different m.c. was evaluated after test. forces. They compared the load–deflection relations lglue between a three-dimensional finite element model and 50 10 experimental results and obtained good agreement. y One can note that experiments have also been performed with the aim of developing design equa- x z tions for glued-in rods, an application that shows strong similarities to FRP overlap joints, see Steiger t=1.4 150 + lglue et al. [5, 6]. In the present study no design parameters are proposed. The objective is rather to investigate the usefulness of various methods for analyzing FRP Fig. 1 The test specimens, 70 9 145 mm2 in cross section, lap joints. One of these is the contact-free evaluation were sawn to 350 mm in length. The FRP was glued to them system just referred to. Two others are the use of using three different anchorage lengths (lglue): 50, 150 and 250 mm analytical models based on generalized Volkersen theory (see [7, 8]), and analysis by use of the finite element method. by means of a spatula. Each FRP was centrically placed on one edge of the wood specimen in question, such that there was 10 mm clearance to the edge of 2 Materials and methods the specimen, see Fig. 1. No clamping was used while attaching the two pieces to each other. 2.1 Test specimens The specimens were of three different types, A, B and C, differing in the length of the overlap, lglue, Wooden test specimens of Norway Spruce 350 mm such that the specimens in the groups had a glued in length were sawn from 5 m long boards 70 9 overlap of 50, 150 and 250 mm, respectively. After 145 mm2 in cross-section. Prior to any further han- the FRP had been glued to the wood, the specimens dling, the wood specimens were stored in a standard were once again stored in the 20°C/65% standard climate at 20°C and a relative humidity of 65% until climate. For each of the three groups, five test moisture equilibrium was achieved. After completion specimens were manufactured, enabling 15 tests to be of the experiments, conducted thereafter, the moisture performed. The part of the FRP sticking out from the content of the wood specimens was verified by oven piece of wood to which it was attached was 150 mm drying and then weighting them. Just prior to the in length in each case. This part of the FRP was used experiments, the surface on the side on which the FRP for applying loads by means of the hydraulic grip of was to be attached by glue was planed. the testing machine. The FRPs were 1.4 mm thick their stiffness and strength, as stated by the manufacturer, were 150 and 2.2 Experimental setup 2000 MPa respectively. All carbon fibres where oriented in the same direction. The FRPs were glued The experimental setup, cf. Fig. 2, aimed at trans- to the wood by use of a 2-component epoxy adhesive mitting shear forces within the plane between the (Resin 220) using an amount of adhesive producing a FRP and the timber. The specimen was fixed on its bond line thickness of 1.3 mm. The glue was applied upper end-grain surface by means of a short steel

Materials and Structures displacement of the piston and utilizing a contact-free measurement system (AramisTM). An obvious differ- ence between the two deformation measurement Grip and loading point methods is that measurements of piston displacement are affected by the flexibility of the setup as a whole Top beam and of the test specimen itself, whereas using the contact-free system displacements between any two Analysis area points within the field of measurements can be for the contact- determined. This latter technique enables the entire free system field of in-plane strains to be measured continuously in the course of an experiment. The contact-free measurement technique is based Steel plate on the use of two cameras which are placed in front of the test object at angles and distances determined by the size of the object and by the lenses involved. With the two cameras, a number of stereoscopic pictures are obtained during testing. The current 3D Fig. 2 Experimental setup. Testing machine. The area eval- position of any point within the measurement field uated by means of the contact-free measurement system is can then be determined by post processing the indicated pictures using the software being a part of the beam having dimensions of 50 9 50 mm2. The beam measurement system. A spray-painted, randomly was held in place and in contact with the specimen by distributed black and white pattern on the surface of use of tie-down threaded rods of the M20 type, the test object, deforming along with the test object together with a washer and a nut. The tie-down rods itself during loading, enables the in-plane strains to were anchored to a solid steel structure (a part of the be assessed. Post-processing of the pictures starts testing machine). The load was applied at the free end with identification of a reference state, here being that of the FRP by displacement-controlled movement, of the unloaded specimen. Each picture is then the displacement increasing successively at 0.5 mm/ subdivided into partially overlapping sections, or min. The loading rate was adjusted so as to lead to facets, the size and amount of overlap being set by failure of the specimen within 1–3 min. The load cell the user on the basis of the spatial resolution and employed had a capacity of 100 kN and a linear accuracy desired. The gray-scale of the pictures is tolerance interval of ±0.1%. An overview of the utilized in performing cross-correlation calculations, setup is shown in Fig. 3. such that each facet position can be tracked with sub- pixel accuracy from one pair of pictures to the next. 2.3 Collection of experimental data This allows different strain measures pertaining from the displacement field to be calculated. Along with registering the force applied by the The frame-grabbing intervals of the two cameras testing machine, deformation data was collected were adjusted so that 50–100 pictures per camera using two different methods: measuring the vertical were obtained during each test. The sampling of the Fig. 3 Overview of the test setup and the data collection Control board for the Load cell ± 100 kN MTS- system. system Volume in which the test specimen is to be placed. CCD- cameras connected to a data-collection and evaluation system.

Materials and Structures load and displacement signals from the testing adhesive layer, b is the width of the adhesive layer, E machine was synchronized in time with the pictures is the modulus of elasticity, and A is the equivalent taken. area in the wood and in the FRPs respectively. The general solution to the differential equation (1) is 2.4 Analytical analysis sð yÞ ¼ C1 coshðxyÞ þ C2 sinhðxyÞ þ sp ð3Þ Analytical models for interaction between wood and The constants C1 and C2 can be calculated using the FRP involving different boundary conditions can be boundary conditions, which for the present case are formulated. A detailed account of how this can be N1(0) = P, N2(0) = -P, N1(L) = 0 and N2(L) = 0. done by use of the generalized Volkersen theory, as it These conditions enable an expression of shear stress, is called, is given by Serrano and Gustafsson [7]. As s(y), to be obtained: shown by e.g. Kirlin [9], the state of stress in the Px coshðxyÞ overlap joint can be mulitaxial. For example stresses sð y Þ ¼ sinhðxyÞ ð4Þ b tanhðxLÞ perpendicular to the loading direction (peel direction) could develop close to the end of the FRP strip. Such This expression can be used to obtain the force N1 by stresses can, in general, be assumed to influence the integration of the shear stress times the width b. level at which failure is initiated, but also the ultimate sinhðxyÞ load level. The generalized Volkersen theory used N1 ð yÞ ¼ P coshðxyÞ ð5Þ here includes only longitudinal shear, although also tanhðxLÞ peel stress could be included in the analysis, for The corresponding strains in the FRP are found to be example by including the shear deformation of the wood, see Gustafsson and Serrano [10]. In order to N1 ð yÞ P sinhðxyÞ e1 ð yÞ ¼ ¼ coshðxyÞ ð6Þ keep the analytical expression as simple as possible, E1 A1 E1 A 1 tanhðxLÞ the 1D-theory is used here, however. This expression implies that, for any given values of Definitions of the symbols used in defining the the load P and of the anchorage length L, the strains specimen and the boundary conditions in question are in the FRP, e1, within the interval 0 B y B L can be shown in Fig. 4. obtained. In the conventional Volkersen theory, [8], the The expressions above are for linear elastic differential equation for the shear stress present in a materials. The so-called generalized Volkersen the- lap joint can be expressed as ory, [7], enables the fracture energy of the bond-line s00 x2 s ¼ 0 ð1Þ to be introduced as an additional parameter. This is done by introducing the equivalentshear stiffness of where the adhesive layer. Accordingly, s2f ð2Gf Þ rather than G/t is used to determine the shear stiffness, where Gf 2 Gb 1 1 x ¼ þ ð2Þ is the fracture energy of the bond line and sf is the t E2 A2 E 1 A1 intrinsic shear strength of the bond line. Introducing In the expressions above, G is the shear stiffness of the equivalent shear stiffness into (1)–(4) and the adhesive layer, t represents the thickness of the assuming that the joint fails when the maximum Fig. 4 Definitions of y=0 y=L y parameters used in the P FRP 1 analytical equations t1 P Thickness of WOOD 2 t2 glue: t

Materials and Structures stress at the most stressed point in the bond line Table 1 Material parameters used in the finite element equals sf allows an expression for the normalized analyses strength of the lap joint to be derived: Material MOE Poissons ratio Pf tanhðxlÞ Wood 10 GPa 0.3 ¼ ð7Þ Asf xl Epoxy, Resin 220 62 MPa a 0.2 where A is the area of the overlap (i.e. A = b 9 lglue). FRP 150 GPa 0.1 For ductile joints, i.e. those in which x approaches a Pertains to the calculated equivalent modulus of elasticity zero, the normalized strength equals unity. This means, in turn, that for such joints the shear stress distribution is uniform. Consequently, the governing since they include possible interface effects in the material parameter for prediction of the load bearing layers between the glue and the wood and between the capacity is the local strength of the bond line, sf. glue and the FRP. In order to keep the model as small as When x is sufficiently large (approaching infinity), possible with respect to the number of degrees of the corresponding ‘‘strength’’ parameter governing freedom, account is taken of the symmetry of the test the load-bearing capacity of the joint is the fracture set-up. The finite element model was loaded by energy of the bond line. Under such conditions, the displacement-controlled movement, the same way that prediction of (7) yields the same result as that it was done in the experiment. The boundary conditions provided by classical linear-elastic fracture mechan- used in the finite element model are shown in Fig. 5. ics theory (LEFM), and the load bearing capacity is Since the main purpose of the current FE-analyses was e.g. independent of the glued length l, but depends on to visualize the general stress distribution along the the ratio of the adherend axial stiffnesses, E1A1/ FRP, and not to estimate a single point maximum stress (E2A2). In cases between the two extreme cases value at e.g. the corners of the FRP, no mesh refinement above, both the local strength and the fracture energy was used in the FE-models. influence the load-bearing capacity of the joint. Thus, the generalized Volkersen theory can be said to be a unifying theory. 3 Results and discussion 2.5 Analysis using the finite element method 3.1 Strength The test specimens were also analyzed numerically The load-bearing capacities obtained from the exper- using the finite element method. Similar analyses iments of each of the fifteen specimens that were have been carried out by Serrano [11], for example, tested, together with the average value obtained for with use of nonlinear FEM. A numerical and each of the three groups, are shown in Table 2. The experimental study of glued-in rods in which strain average value for groups A, B and C i.e. for anchorage distributions similar to those achieved in the present lengths 50, 150 and 250 mm, were 18.4, 32.8 and study has been carried out by del Senno et al. [12]. 35.5 kN, respectively. This shows clearly that the In order to perform the present analysis six material load-bearing capacity depends on the anchorage parameters, two for each material, were introduced length, although in a non-linear fashion, and that under the assumption of the material being linear- the influence of the anchorage length diminishes as elastic isotropic, see Table 1. This is obviously an the anchorage length increases. The highest load- approximation since wood, for example, is normally bearing capacity was that obtained for group C, which considered to be a strongly orthotropic material, yet for had the greatest anchorage length, however in group the analysis here the approximation is quite adequate, B, having an anchorage length 40% less, the strength since the load is introduced primarily in the longitu- is only 7.6% lower. In addition, in group A the dinal direction of the wood. The accuracy of the anchorage length is 20% that of the anchorage length FE-model was verified by use of models involving in group C, whereas the load-bearing capacity for that orthotropic parameters. The properties that are given group is nearly 50% of that obtained for group C. In for the glue should be considered as equivalent values Fig. 6 the average strength is shown as a function

Materials and Structures Fig. 5 Boundary B.C. used in the FE- analysis. conditions and loading of [mm] the finite element model Front view Side view used for simulation of the lap-joint 145 70 Wood 350 FRP lglue 50 150 + lglue t=1.4 Displacement controlled loading. 40 Table 2 Load-bearing capacities obtained for specimens within groups A, B and C and the mean value for each group 35 Group A B C 30 Average strength [kN] Anchorage length 50 mm 150 mm 250 mm 25 Test specimen 1 16.9 31.5 33.7 20 2 20.3 36.9 36.6 15 3 16.4 31.9 36.5 4 18.8 32.4 35.5 10 5 19.4 31.1 35.4 5 Average load-bearing capacity 18.4 32.8 35.5 0 The values are given in kN 0 50 100 150 200 250 300 Anchorage length [mm] of the anchorage length, highlighting the highly Fig. 6 Average of experimentally obtained results for anchor- non-linear nature of this relation. age lengths 50, 150 and 250 mm respectively Two different failure modes were found to occur in the experiment, one of these being shear failure of The normalized strength of a joint as a function of the wood material and the other a combination of the anchorage length is shown in Fig. 8. The analytical failure of the wood and of the adhesive at the solution has been fitted to the experimentally obtained interface between the FRP and glue. An example of result in a least square sense, by varying the shear each of these two modes is shown in Fig. 7. Most strength sf and the fracture energy Gf. The fit to the common for all three different anchorage lengths was analytical solution yielded a value of 8.2 MPa for the shear failure of the wood material. the shear strength and 1700 Nm/m2 for the fracture

Materials and Structures Fig. 7 An example of each of the two failure modes that appeared: a shear failure of the wood material (test specimen A3), b combination of shear failure of the wood and adhesive failure at the junction of wood fibre and epoxy (test specimen C3) joint for shorter than for longer anchorage lengths. The 1 shape of the curve follows closely the three mean results of the experiments. Note that more experiments Normalized strength [-] 0.8 should be performed in order to verify the curve for longer anchorage lengths, those longer than around 0.6 300 mm. The results agree well with results previously obtained by e.g. Johansson et al. [2] and Steiger et al. 0.4 [5]. 0.2 3.2 Stiffness 0 Figure 9 shows the load–displacement response 0 50 100 150 200 250 300 350 400 Anchorage length [mm] obtained in the tests. Curves based on displacement as measured by the vertical displacement of the Fig. 8 Normalized strength of the joint as a function of the piston and as well as curves based on displacement as anchorage length. The analytical expression (8) is shown as a measured by the contact-free system are shown. solid line and the measured normalized strength for each of the three groups A, B and C is marked with an asterisk Using the curves based on the vertical displacement of the piston, the stiffness can be calculated to be energy. The effective area in the wood was assumed to approximately 30 MN/m. This value is independent be 50 mm wide and 50 mm deep, as based on the width of the anchorage length. The differences between the of the FRP and the depth of the top beam. The curve plotted curves can be partly explained in terms of shows a given change in anchorage length to have a local phenomena in the test setup. In the curves based stronger influence on the normalized strength of the on the vertical movement of the piston those effects

Materials and Structures Fig. 9 Load–displacement 40 curves for all 15 specimens when the vertical 35 displacement is measured in the piston and for eight of 30 the specimens when the vertical displacement is 25 Load [kN] obtained from the contact- free (c-f) system 20 15 A1 A2 A3 A4 A5 B1 B2 B3 10 B4 B5 C1 C2 C3 C4 C5 A1 c-f 5 A2 c-f A3 c-f B1 c-f B2 c-f B3 c-f C2 c-f C3 c-f 0 0 0,5 1 1,5 2 Displacement [mm] vertical displacement from vertical displacement the contact-free system from the piston will be included in contradiction to the curves based on the contact-free system. FRP In order to avoid inclusion of the flexibility of the test set-up in measuring the lap-joint stiffness, test specimen numbers 1, 2 and 3 in each group were [mm] evaluated with respect to the relative vertical dis- P2 placement between a point P1 located on the piece of ~10 P1 wood 10 mm from the upper edge and a point P2 35 located in the center of the FRP on the edge of the wood piece, see Fig. 10. This was easily done by 25 use of the optical evaluation system. The relation between the load and this relative displacement, y together with the load and vertical displacements as obtained from the piston, are shown in Fig. 9. For the case in which the distance between the two points is Line 1 employed, the stiffness obtained is about 180 kN/m, some six times as high as when the vertical position x of the piston is the basis for the calculations. This WOOD difference highlights the power of using an optical system with the possibilities it provides of selecting Fig. 10 Definitions of points P1 and P2 between which evaluation points after testing has been performed. vertical displacements were measured, and Line 1, along The accuracy of testing can be markedly increased in which the strain component ey was measured this way. of the three cases shows the results obtained for a 3.3 Strain distribution given load from the contact-free system, the bottom part of the respective figure showing the results of the It can be shown from results obtained using the finite element analysis for the same load. The red contact-free system how the strain (ey) varies over a colour indicates large strains and the blue colour given specimen. Figure 11 presents an example from small to negative strains. It can be readily seen that each of the three groups of how strain is distributed in the strains in the FRP are largest close to the edge of a test specimen. The upper part of the figure in each the piece of wood, their decreasing then toward in the

Materials and Structures Fig. 11 Examples of strains ey close to failure obtained in one of the testings in each of the three groups. ey for a test specimen from group A, F = 16.6 kN; ey for a test specimen from group B, F = 32.2 kN; ey for a test specimen from group C, F = 36.6 kN inner parts of the glued area. For group A it can also maximum strain just prior to failure was 1.45% for be seen that the strains are largest in the part of the group A, 2.80% for group B and 2.81% for group C. wood toward the end of the FRP. The figure shows that the normal strains (in the In Fig. 12 the normal strains in the FRP along line FRP) at the edge are appreciably lower in group A 1, defined as in Fig. 10, obtained in three different than in groups B and C, where they are quite similar ways are compared with each other for group A, B in size. The relatively linear strain distribution can be and C respectively. The strains shown are those explained by the fact that the glue is of relatively low obtained by use of the contact-free measurement stiffness compared with the material it is glued to. A system, as well as on the basis of the analytical perfectly linear distribution would imply that the expression and the numerical FE-analysis. The strains shear stress in the bond line is constant along the obtained in the experiments were averaged within overlap. The analytical calculations, as previously each group before being plotted in the figure. The indicated, are based for each of the specimens on an Fig. 12 Moving average of 4,00 the component ey in the FRP Grupp A - experimental at maximum load within Grupp B - experimental each group. The analytical 3,00 Grupp C - experimental results and the results of the Grupp A - analytical Milli strain [-] finite element analysis are Grupp B - analytical also shown for each of the Grupp C - analytical 2,00 three groups Grupp A - FEM Grupp B - FEM Grupp C - FEM 1,00 0,00 0 20 40 60 80 100 120 140 160 180 200 220 240 Anchorage length [mm]

Materials and Structures effective area of 50 9 50 mm2 and a glue thickness – The load-bearing capacity of the joint is partly a of t = 1.3 mm. The equivalent shear modulus G of function of the anchorage length, becoming the glue can be calculated as having a value of greater if the anchorage length is increased, but 25.7 MPa according to the formula beyond a certain point the anchorage length appears to play only a limited role. In the s2f t G¼ ð8Þ experiments carried out, this was shown by the 2Gf fact that, despite there being about a 40% where the shear strength sf = 8.2 MPa and the difference in anchorage length between groups fracture energy Gf = 1700 Nm/m2. The results of B and C, the average strength of the two differed the three-dimensional FE-analysis are also shown in by only about 10%. Fig. 12. A thickness of t = 1.3 mm was used for the – The strain was found to be at a maximum at a glue, the corresponding modulus of elasticity being point close to the end of the piece of wood. The calculated as 62 MPa (corresponding to a G = maximum strain measured prior to failure was 25.7 MPa and a Poisson’s ratio of m = 0.2). The 1.45% for group A, 2.80% for group B and agreement between the calculations and the results of 2.81% for group C (average values). the experiments is rather close, implying that calcula- – For the type of lap-joints involved, close agree- tions for the type of lap joints shown here can be done ment between results of the experiments and analytically using generalized Volkersen theory and results based on use of generalized Volkersen numerically using linear FEM. theory as well as of linear FE-analysis was obtained. An important aspect of the analyses carried out was to introduce the bond-line fracture 4 Conclusions energy as a major parameter. – The load-bearing capacity of joints of the type The 15 test specimens, in each of which a 50 mm studied depends on the local strength of the bond wide and 1.4 mm thick laminate of reinforced fibre line, the geometry of the joint (anchorage length polymers was glued to a 70 mm wide piece of wood, and cross sectional area of the adherends) the were all loaded to failure. The specimens belonged to stiffness of the FRP and the wood, and on the three different groups, those having a 50, 150 and fracture energy of the bond line. 250 mm long anchorage, respectively, of the FRP to Gluing FRPs to timber can increase both the strength the wood. The deformation and the stiffness of the and the stiffness of parts of a structure in which this is joints were evaluated using an optical evaluation needed. In the experiments carried out, the effects of system. The load-bearing capacity, the stiffness and different anchorage lengths as well as of certain the strains were also evaluated using both analytical critical strains were examined. The close agreement expressions and numerical methods. The results of obtained between the theoretical calculations and the experimental investigation and of the numerical results of the tests performed show it to be possible to and the analytical calculations allow a number of perform simulations in this area with a high degree of conclusions to be drawn. accuracy. – The stiffness of the joints within the interval Acknowledgements The authors want to express their that was tested is basically independent of the sincere gratitude to Såg i Syd for the financial support to the anchorage length. For the combination of FRP, studies. glue and wood examined the stiffness was found to be 180 MN/m. References – To obtain an accurate stiffness value it is important that only the stiffness of the part that 1. Gustafsson P, Enquist B (1993) Advanced materials based is studied be assessed. If a contact-free optical on straw and wood Fibre reinforcement of glulam. Division evaluation system is employed, the part to be of Structural Mechanics, Lund University, Lund 2. Johansson H, Blanksvärd T, Carolin A (2006) Glulam studied can readily be chosen after the experiment members strengthened by carbon fibre reinforcement. has been carried out. Mater Struct 40:47–56

Materials and Structures 3. Kliger R, Johansson M, Crocetti R (2008) Strengthening 9. Kirlin CP (1996) Experimental and finite-element analysis timber with CFPR or steel plates—short and long-term of stress distribution near the end of reinforcement in par- performance. In: World conference on timber engineering, tially reinforced glulam. MS thesis, Department of Wood Miyazaki, Japan Science & Engineering, Oregon State University, Corvallis 4. Guan ZW, Rodd PD, Pope DJ (2005) Study of glulam 10. Gustafsson PJ, Serrano E (2002) Glued-in rods for timber beams pre-stressed with pultruded GRP. Comput Struct 83: structures—development of a calculation model. Report 2476–2487 TVSM-3056. Division of Structural Mechanics, Lund Uni- 5. Steiger R, Gehri E, Widmann R (2006) Pull-out strength of versity, Lund axially loaded steel rods bonded in glulam parallel to the 11. Serrano E (2000) Adhesive joints in timber engineering— grain. Mater Struct 40:69–78 modelling and testing of fracture properties. Report TVSM 6. Steiger R, Gehri E, Widmann R (2004) Glued-in steel rods: 1012. PhD-thesis, Department of Mechanics and Materials, a design approach for axially loaded single rods set parallel Lund University, Lund to the grain. In: CIB-W18 meeting thirty-seven, Edinburgh, 12. del Senno M, Piazza M, Tomasi R (2004) Axial glued-in UK steel timber joints—experimental and numerical analysis. 7. Serrano E, Gustafsson P (2006) Fracture mechanics in Holz als Roh- und Werkstoff 62:137–146 timber engineering—strength analyses of components and joints. Mater Struct 40:87–96 8. Volkersen O (1938) Die Nietkraftverteilung in zug- beanspruchten Nietverbindungen mit konstanten Laschen- querschnitten. Luftfahrtforschung 15:41–47

You can also read